Presentation on theme: "I F CANNOT BEAR SUCH CONDITIONS … 1 Sub-topics Failure Ductile and brittle fracture Fracture toughness Fundamentals of fracture mechanics."— Presentation transcript:
I F CANNOT BEAR SUCH CONDITIONS … 1 Sub-topics Failure Ductile and brittle fracture Fracture toughness Fundamentals of fracture mechanics
F AILURE An oil tanker that fractured in a brittle manner by crack propagation around its girth. ( Photography by Neal Boenzi. Reprinted with permission from The New York Times.) Failure in structures leads to lost of properties and sometimes lost of human lives. 2
T YPES OF FRACTURE Fracture is the separation of a body into two or more pieces in response to an imposed stress that is static and at temperatures that are low relative to the melting temperature of the material. 3
F AILURE MODES Moderately ductile fracture after some necking. Brittle fracture without any plastic deformation. Highly ductile fracture in which the specimen necks down to a point 4 Ductile fracture is almost always preferred to brittle one.
D UCTILE FRACTURE Highly ductile fracture in which the specimen necks down to a point 5
D UCTILE FRACTURE Cup-and-cone fracture in aluminum. Final shear fracture. Initial necking. Small cavity formation Coalescence of cavities to form a crack C rack propagation 6
T OUGH “ DUCTILE ” FRACTURE Ductile fracture is a much less serious problem in engineering materials since failure can be detected beforehand due to observable plastic deformation prior to failure. Under uniaxial tensile force, after necking, microvoids form and coalesce to form crack, which then propagate in the direction normal to the tensile axis. The crack then rapidly propagate through the periphery along the shear plane, leaving the cub and cone fracture. 7
M ICROVOID FORMATION, GROWTH AND COALESCENCE Microvoids are easily formed at inclusions, intermetallic or second-phase particles and grain boundaries. Growth and coalescence of microvoids progress as the local applied load increases. Random planar array of particles acting as void initiators Growth of voids to join each other as the applied stress increases. Linkage or coalescence of these voids to form free fracture surface. 8
D UCTILE FRACTURE OF ALLOYS 9 If materials is stretched, it firstly deforms uniformly. Inclusions – stress concentrators
F ORMATION OF MICROVOIDS FROM SECOND PHASE PARTICLES 1) Decohesion at particle - matrix interface. 2) Fracture of brittle particle 3) Decohesion of an interface associated with shear deformation or grain boundary sliding. Decohesion of carbide particles from Ti matrix. Fractured carbides aiding microvoid formation. 10
B RITTLE FRACTURE 11
F RACTOGRAFIC STUDIES Scanning electron fractograph of ductile cast iron showing a transgranular fracture surface. Scanning electron fractograph showing an intergranular fracture surface. 12
N ATURE OF FRACTURE : BRITTLE Characteristic for ceramics and glasses Distinct characteristics of brittle fracture surfaces: 1) The absence of gross plastic deformation. 2) Grainy or Faceted texture. 3) “River” marking or stress lines. 13
I NTERGRANULAR FRACTURE Intergranular failure is a moderate to low energy brittle fracture mode resulting from grain boundary separation or segregation of embrittling particles or precipitates. Embrittling grain boundary particles are weakly bonded with the matrix, high free energy and unstable, which leads to preferential crack propagation path. Intergranular fracture with and without microvoid coalescence 14
S TRENGTH AND TOUGHNESS 15 Strength Resistance of a material to plastic flow Toughness Resistance of a material to the propagation of a crack How concerned should you be if you read in the paper that cracks have been detected in the pressure vessel of the nuclear reactor of the power station a few miles away?
T ESTING FOR TOUGHNESS This type of test provides a comparison of the toughness of materials – however, it does not provide a way to express toughness as a material property (no true material property that is independent on size and shape of the test sample) Tear test Impact test Measuring the energy 16
I NTRODUCTION TO FRACTURE MECHANICS The fracture strength of a solid material is a function of the cohesive forces that exist between atoms. On this basis, the theoretical cohesive strength of a brittle elastic solid has been estimated to be approximately E/10, where E is the modulus of elasticity. The experimental fracture strengths of most engineering materials normally lie between 10 and 1000 times below this theoretical value. Why? surface energy unstrained interatomic spacing 17
S TRESS CONCENTRATION Crack reduces the cross – section => increase in stress What will happen with tough material? Cracks concentrate stress Flaws are detriment to the fracture strength because an applied stress may be amplified or concentrated at the tip, the magnitude of this amplification depends on crack orientation and geometry. 18
W HAT FORCE IS REQUIRED TO BREAK THE SAMPLES ? 19
T HEORIES OF BRITTLE FRACTURE 20
S TRESS CONCENTRATORS Schematic stress profile along the line X–X the magnitude of this localized stress diminishes with distance away from the crack tip The maximum stress at the crack tip stress concentration factor A measure of the degree to which an external stress is amplified at the tip of a crack 21
P ROBLEM Consider a circular hole in a plate loaded in tension. When will material near the hole yield? 2. A plate with a rectangular section 500 mm by 15 mm carries a tensile load of 50kN. It is made of a ductile metal with a yield strength of 50 MPa. The plate contains an elliptical hole of length 100 mm and a minimum radius of 1 mm, oriented as shown in the diagram. What is (a) the nominal stress (b) The maximum stress in the plate? (c) Will the plate start to yield? (d) Will it collapse completely?
T HEORETICAL STRESS CONCENTRATION FACTOR CURVES 23
G RIFFITH THEORY OF BRITTLE FRACTURE Inherent defects in brittle materials lead to stress concentration. 24 If stress exceeds the cohesive strength of bonds, crack extension is possible. Thermodynamic criterion: There are two energies to be taken into account when a crack propagates: (1)New surfaces should be created and a certain amount of energy must be provided to create them; (2)Elastic strain energy stored in the stressed material is released during crack propagation.
T HEORY OF BRITTLE FRACTURE 25 The stress required to create the new crack surface Critical stress for crack propagation The strain energy release rate (G) is higher for higher loads and larger cracks. If the strain energy released exceeds a critical value, then the crack will grow spontaneously. For brittle materials, stress can be equal to the surface energy of the (two) new crack surfaces; in other words, in brittle materials, a crack will grow spontaneously if the strain energy released is equal to or greater than the energy required to grow the crack surface(s). The stability condition can be written as elastic energy released (G) = surface energy created (2γ) If the elastic energy release is less than the critical value, the crack will not grow. G ≥ 2γ
P ROBLEM A relatively large plate of a glass is subjected to a tensile stress of 40 MPa. If the specific surface energy and modulus of elasticity for this glass are 0.3 J/m2 and 69 GPa, respectively, determine the maximum length of a surface flaw that is possible without fracture. 26
P ROBLEM : P ROPERTIES OF S I A L ON C ERAMICS 27 Assume that an advanced ceramic, SiAlON (silicon aluminum oxynitride), has a tensile strength of 414 MPa. Let us assume that this value is for a flaw-free ceramic. (In practice, it is almost impossible to produce flaw-free ceramics.) A crack cm deep is observed before a SiAlON part is tested. The part unexpectedly fails at a stress of 3.5 MPa by propagation of the crack. Estimate the radius of the crack tip.
BASIC MODES OF CRACK TIP DEFORMATION K IC – the critical stress intensity in mode I fracture (plain strain) critical stress for crack propagation 28 K = (EG) 1/2
F RACTURE TOUGHNESS FT is a material property ; Value is independent of the way it is measured; Can be used for design Fracture toughness of a material is obtained by determining the ability of a material to withstand the load in the presence of a sharp crack before failure. Y is a dimensionless parameter or function that depends on both crack and specimen sizes and geometries, as well as the manner of load application 29 Crack propagates when the stress intensity factor exceeds a critical value.
E NERGY RELEASE RATE Irwin later modified the Griffith theory by replacing the term 2γ with the potential strain energy release rate G When a samples fractures, a new surface is created => necessary conditions for fracture – sufficient energy release G≥ 2γ The critical condition to which the crack propagates to cause global failure is when this G value exceeds the critical value Irwin showed that G is measurable and can be related to the stress intensity factor, K 30
Y VALUES OF VARIOUS CRACK GEOMETRIES 31
P ROCESS ZONE A plastic zone forms at the crack tip where the stress would otherwise exceed the yield strength Size of process zone: 32
B RITTLE “ CLEAVAGE ” FRACTURE Materials of high yield strength Near tip stress are very high => tear the atomic bonds apart => increase in the crack length results in increase in K, causing crack to accelerate 33
F RACTURE TOUGHNESS AND DESIGN If the K IC value of material is known and the presence of a crack is allowed, we can then monitor the crack propagation during service prior to failure => How long we can use the component before it fails. Brittle materials, for which appreciable plastic deformation is not possible in front of an advancing crack, have low KIc values and are vulnerable to catastrophic failure. 34 Crack length necessary for fracture at a materials yield strength
Tough metals are able to contain large cracks but still yield in a predictable, ductile, manner Critical crack lengths are a measure of the damage tolerance of a material D AMAGE TOLERANCE 35
F RACTURE RESISTANCE The ability of a material to resist the growth of a crack depends on a large number of factors: Larger flaws reduce the permitted stress. The ability of a material to deform is critical. Increasing the rate of application of the load, such as that encountered in an impact test, typically reduces the fracture toughness of the material. Increasing the temperature normally increases the fracture toughness. 36
F RACTURE TOUGHNESS – MODULUS CHART Values range from 0.01 – 100 MPa√m 38
39 Transition crack length plotted on chart – values can range from near- atomic dimensions for ceramics to almost a meter for ductile metals
F AIL -S AFE D ESIGN Yield-before-break Requires that the crack will not propagate even if the stress causes the part to yield Leak-before-break Requires that a crack just large enough to penetrate both the inner and outer surface of the vessel is still stable 40
D ESIGN USING FRACTURE MECHANICS Consider the thin-walled spherical tank of radius r and thickness t that may be used as a pressure vessel. One design of such a tank calls for yielding of the wall material prior to failure as a result of the formation of a crack of critical size and its subsequent rapid propagation. Thus, plastic distortion of the wall may be observed and the pressure within the tank released before the occurrence of catastrophic failure. Consequently, materials having large critical crack lengths are desired. On the basis of this criterion, rank the metal alloys listed in Table, as to critical crack size, from longest to shortest. wall stress 41
D ESIGN PROCESS – YIELD - BEFORE - FRACTURE 42 Requirement : The stresses are everywhere less that required to make a crack of critical length to propagate. BUT!!! It is not safe… Requirement : Crack should not propagate even if the stress is sufficient to cause general yield – for then the vessel will deform stably in a way that can be detected. ≤ Tolerable crack size
D ESIGN PROBLEM - LEAK - BEFORE - BREAK An alternative design that is also often utilized with pressure vessels is termed leak-before-break. Using principles of fracture mechanics, allowance is made for the growth of a crack through the thickness of the vessel wall prior to the occurrence of rapid crack propagation. Thus, the crack will completely penetrate the wall without catastrophic failure, allowing for its detection by the leaking of pressurized fluid. With this criterion the critical crack length a c (i.e., one-half of the total internal crack length) is taken to be equal to the pressure vessel thickness t. Using this criterion, rank the metal alloys in Table as to the maximum allowable pressure. 43 2a = t ≤
F ORENSIC FRACTURE CASE 44 K 1c of the tank material measured to be 45 MPa√m 10 mm crack found in longitudinal weld Stress based on maximum design pressure Stress at which a plate with the given K 1c will fail with a 10 mm crack
D ESIGN OF A CERAMIC SUPPORT 45 Determine the minimum allowable thickness for a 7.5 cm wide plate made of sialon (SiAlON or silicon aluminumoxynitride) that has a fracture toughness of 9.9 Mpa m 1/2. The plate must withstand a tensile load of N. The part will be non-destructively tested to ensure that no flaws are present that might cause failure. The minimum allowable thickness of the part will depend on the minimum flaw size that can be determined by the available testing technique. Assume that three non-destructive testing techniques are available: X-ray radiography can detect flaws larger than 0.05 cm; gamma-ray radiography can detect flaws larger than 0.02 cm; and ultrasonic inspection can detect flaws larger than cm. Assume that the geometry factor f = 1.0 for all flaws.
D UCTILE - TO -B RITTLE TRANSITION At low temperatures some metals and all polymers become brittle As temperatures decrease, yield strengths of most materials increase leading to a reduction in the plastic zone size Only metals with an FCC structure remain ductile at the lowest temperatures 46 The ductile to brittle transition temperature is the temperature at which the failure mode of a material changes from ductile to brittle fracture.
D UCTILE TO BRITTLE TRANSITION BEHAVIOUR Some metals and polymers experience ductile-to-brittle transition behaviour when subjected to decreasing temperature, resulting from a strong yield stress dependence on temperature. Metals possess limited slip systems available at low temperature, minimising the plastic deformation during the fracture process. Increasing temperature allows more slip systems to operate, yielding general plastic deformation to occur prior to failure. 47
W HEN DUCTILE TURN TO BRITTLE The criterion for a material to change its fracture behaviour from ductile to brittle mode is when the yield stress at the observed temperature is larger than the stress necessary for the growth of the micro-crack indicated in the Griffith theory The criterion for ductile to brittle transition is when the term on the left hand side is greater than the right hand side. τ is the lattice resistance to dislocation movement k’ is a parameter related to the release of dislocation into a pile-up D is the grain diameter (associated with slip length). G is the shear modulus β is a constant depending on the stress system 48
W HY DON ’ T SOME MATERIALS UNDERGO TRANSITION ? Unlike steel, aluminium does not undergo a ductile-brittle transition. The reason can be explained in terms of their crystal structure. The yield stress of steel is temperature sensitive because of its BCC structure. At low temperatures it is more difficult for the dislocations to move (they require a degree of diffusion to move due to the non-close packed nature of the slip planes) and therefore plastic deformation becomes more difficult. The effect of this is to increase the yield stress at low temperatures. Aluminium has a FCC structure, this means that it has lots of easily operated close-packed slip systems operating at low temperatures. As a result its yield strength is not temperature sensitive and aluminium remains ductile to low temperatures. 49
B AD LUCK OF “T ITANIC ” The sinking of the “Titanic” was caused primarily by the brittleness of the steel used to construct the hull of the ship. In the icy water of the Atlantic, the steel was below the ductile to brittle transition temperature. 50
F ACTORS AFFECTING MODES OF FRACTURE The yield stress of steel is temperature sensitive. The fracture stress remains relatively constant with temperature. At room temperature steel is a ductile material, this means that it will undergo plastic deformation before fracture i.e. the yield strength of the material is less than the fracture stress.ductile At low temperatures the yield stress of steel increases, when the yield stress increases above the fracture stress the material will undergo a ductile-to-brittle transition. 51
T HE S TRENGTH -T OUGHNESS TRADE - OFF Increasing the yield strength of a metal decreasing the size of the plastic zone surrounding a crack – this leads to decreased toughness 52
M ETALLURGICAL ASPECT OF FRACTURE Microstructure in metallic materials are highly complex. Various microstructural features affect how the materials fracture There are microstructural features that can play a role in determining the fracture path, the most important are High strength materials usually possess several microstructural features in order to optimise mechanical properties by influencing deformation behaviour / fracture paths. 53